#------------------------------------------------------------------------------
#$Date: 2015-07-05 10:34:00 +0300 (Sun, 05 Jul 2015) $
#$Revision: 140058 $
#$URL: svn://www.crystallography.net/cod/cif/4/51/29/4512948.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4512948
loop_
_publ_author_name
'Amanchi, Srinivasa Rao'
'Khenkin, Alexander M.'
'Diskin-Posner, Yael'
'Neumann, Ronny'
_publ_section_title
;
 Bismuth-Substituted “Sandwich” Type Polyoxometalate
 Catalyst for Activation of Peroxide: Umpolung of the Peroxo Intermediate
 and Change of Chemoselectivity
;
_journal_issue                   6
_journal_name_full               'ACS Catalysis'
_journal_page_first              3336
_journal_paper_doi               10.1021/acscatal.5b00066
_journal_volume                  5
_journal_year                    2015
_chemical_formula_moiety         'Bi2 O68 W18 Zn4, 2(O2 Zn), 26.56(O), 4(Na)'
_chemical_formula_sum            'Bi2 Na4 O98.55 W18 Zn6'
_chemical_formula_weight         5788.24
_space_group_crystal_system      orthorhombic
_space_group_IT_number           58
_space_group_name_Hall           '-P 2 2n'
_space_group_name_H-M_alt        'P n n m'
_symmetry_space_group_name_Hall  '-P 2 2n'
_symmetry_space_group_name_H-M   'P n n m'
_audit_creation_method           SHELXL-2014/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   16.187(3)
_cell_length_b                   19.430(4)
_cell_length_c                   14.641(3)
_cell_measurement_reflns_used    9100
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      26.37
_cell_measurement_theta_min      1.98
_cell_volume                     4604.8(16)
_computing_cell_refinement       HKL
_computing_data_collection       'Collect package Nonius'
_computing_data_reduction        HKL
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      120(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Nonius KappaCCD'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0258
_diffrn_reflns_av_unetI/netI     0.0241
_diffrn_reflns_laue_measured_fraction_full 0.994
_diffrn_reflns_laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            4891
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.369
_diffrn_reflns_theta_min         3.388
_exptl_absorpt_coefficient_mu    27.850
_exptl_absorpt_correction_T_max  0.3365
_exptl_absorpt_correction_T_min  0.1496
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'Nonius KappaCCD'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.175
_exptl_crystal_description       prism
_exptl_crystal_F_000             5021
_exptl_crystal_size_max          0.110
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.050
_refine_diff_density_max         2.586
_refine_diff_density_min         -3.480
_refine_diff_density_rms         0.368
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.063
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     341
_refine_ls_number_reflns         4891
_refine_ls_number_restraints     19
_refine_ls_restrained_S_all      1.065
_refine_ls_R_factor_all          0.0499
_refine_ls_R_factor_gt           0.0423
_refine_ls_shift/su_max          0.022
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0669P)²+90.1528P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1119
_refine_ls_wR_factor_ref         0.1153
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4243
_reflns_number_total             4891
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cs5b00066_si_002.cif
_cod_data_source_block           n421
_cod_depositor_comments
'Adding full bibliography for 4512947--4512948.cif.'
_cod_database_code               4512948
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.150
_shelx_estimated_absorpt_t_max   0.336
_shelxl_version_number           2014/6
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'x-1/2, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
W1 W 0.66367(3) 0.40011(3) 0.12757(4) 0.03120(15) Uani 1 1 d . . .
W2 W 0.73145(4) 0.24377(3) 0.0000 0.02655(17) Uani 1 2 d S T P
W3 W 0.84410(3) 0.40398(2) 0.23458(3) 0.02751(14) Uani 1 1 d . . .
W4 W 0.77747(3) 0.54082(2) 0.12924(4) 0.03033(15) Uani 1 1 d . . .
W5 W 0.90846(3) 0.24573(2) 0.11132(3) 0.02539(14) Uani 1 1 d . . .
Zn1 Zn 0.85882(12) 0.40090(8) 0.0000 0.0193(4) Uani 1 2 d S T P
Zn2 Zn 1.0000 0.5000 0.10844(11) 0.0210(4) Uani 1 2 d S T P
Bi1 Bi 0.93011(4) 0.63907(3) 0.0000 0.02415(16) Uani 1 2 d S T P
O1 O 0.5622(6) 0.3875(5) 0.1623(7) 0.043(2) Uani 1 1 d . . .
O2 O 0.6504(8) 0.1856(7) 0.0000 0.034(3) Uani 1 2 d S T P
O3 O 0.8543(6) 0.3895(4) 0.3517(6) 0.036(2) Uani 1 1 d . . .
O4 O 0.7462(6) 0.6206(5) 0.1680(7) 0.040(2) Uani 1 1 d . . .
O5 O 0.9392(6) 0.1854(4) 0.1911(6) 0.032(2) Uani 1 1 d . . .
O6 O 0.6932(5) 0.3093(4) 0.0888(6) 0.0283(18) Uani 1 1 d . . .
O7 O 0.6478(7) 0.4170(6) 0.0000 0.031(3) Uani 1 2 d S T P
O8 O 0.7170(6) 0.3842(4) 0.2398(6) 0.033(2) Uani 1 1 d . . .
O9 O 0.6658(5) 0.4982(5) 0.1448(6) 0.034(2) Uani 1 1 d . . .
O10 O 0.7963(5) 0.2023(4) 0.0941(5) 0.0235(16) Uani 1 1 d . . .
O11 O 0.9397(8) 0.1951(6) 0.0000 0.028(3) Uani 1 2 d S T P
O12 O 0.8549(5) 0.3107(4) 0.1922(5) 0.0259(17) Uani 1 1 d . . .
O13 O 0.8049(6) 0.5012(4) 0.2486(5) 0.033(2) Uani 1 1 d . . .
O14 O 0.7524(7) 0.5491(6) 0.0000 0.026(2) Uani 1 2 d S T P
O15 O 0.8520(7) 0.3005(5) 0.0000 0.021(2) Uani 1 2 d S T P
O16 O 0.7948(5) 0.4317(4) 0.1047(5) 0.0233(17) Uani 1 1 d . . .
O17 O 1.0021(5) 0.6991(4) -0.1051(5) 0.0240(17) Uani 1 1 d . . .
O18 O 0.9428(5) 0.4338(4) 0.2022(5) 0.0237(17) Uani 1 1 d . . .
O19 O 0.8886(5) 0.5538(4) 0.1055(5) 0.0262(18) Uani 1 1 d . . .
O20 O 1.0273(7) 0.5691(5) 0.0000 0.022(2) Uani 1 2 d S T P
Zn3 Zn 0.7029(3) 0.50482(19) 0.5000 0.0553(9) Uani 0.8 2 d S TU P
Zn3A Zn 0.6474(14) 0.4740(11) 0.5000 0.082(5) Uiso 0.2 2 d S . P
Na1 Na 0.5689(7) 0.5419(5) 0.2822(7) 0.106(3) Uani 1 1 d . . .
O21 O 0.7246(11) 0.2393(5) 0.2540(11) 0.072(6) Uani 0.89(4) 1 d . U P
O22 O 0.785(3) 0.0609(12) 0.1121(14) 0.030(9) Uani 0.46(7) 1 d . . P
O22A O 0.747(2) 0.0718(11) 0.0977(14) 0.028(6) Uiso 0.54(7) 1 d . . P
O23 O 0.8120(15) 0.4568(9) 0.5000 0.078(6) Uani 1 2 d S T P
O24 O 0.6551(12) 0.4376(11) 0.5968(11) 0.050(7) Uani 0.56(3) 1 d . . P
O24A O 0.6124(17) 0.3973(13) 0.6175(17) 0.049(9) Uiso 0.44(3) 1 d . . P
O25 O 0.5532(14) 0.5563(12) 0.0000 0.116(10) Uani 1 2 d S T P
O26 O 0.5648(17) 0.5531(10) 0.5000 0.106(8) Uani 1 2 d S TU P
O27 O 0.5668(18) 0.084(3) 0.172(4) 0.063(15) Uani 0.46(10) 1 d . U P
O27A O 0.570(2) 0.055(3) 0.146(3) 0.072(11) Uiso 0.54(10) 1 d . . P
O28 O 0.575(2) 0.2118(17) 0.2138(19) 0.224(15) Uani 1 1 d . . .
O29 O 0.471(3) 0.141(2) 0.0000 0.089(13) Uani 0.5 2 d S TU P
O30 O 0.629(2) 0.2975(15) 0.5000 0.187(17) Uani 1 2 d S T P
O31 O 0.6047(12) 0.0750(9) 0.0000 0.021(4) Uani 0.6 2 d S T P
O31A O 0.6634(19) 0.0583(15) 0.0000 0.025(6) Uiso 0.4 2 d S . P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O8 98.9(5) . .
O1 W1 O7 100.5(5) . .
O8 W1 O7 160.4(4) . .
O1 W1 O6 101.1(4) . .
O8 W1 O6 89.6(4) . .
O7 W1 O6 84.4(4) . .
O1 W1 O9 96.8(4) . .
O8 W1 O9 92.3(4) . .
O7 W1 O9 87.8(4) . .
O6 W1 O9 161.5(3) . .
O1 W1 O16 168.8(4) . .
O8 W1 O16 75.0(3) . .
O7 W1 O16 86.2(4) . .
O6 W1 O16 88.4(3) . .
O9 W1 O16 74.4(3) . .
O2 W2 O10 98.1(4) . 6
O2 W2 O10 98.1(4) . .
O10 W2 O10 92.3(5) 6 .
O2 W2 O6 100.8(4) . 6
O10 W2 O6 88.2(3) 6 6
O10 W2 O6 160.8(3) . 6
O2 W2 O6 100.9(4) . .
O10 W2 O6 160.8(3) 6 .
O10 W2 O6 88.2(3) . .
O6 W2 O6 85.1(5) 6 .
O2 W2 O15 168.7(5) . .
O10 W2 O15 74.3(3) 6 .
O10 W2 O15 74.3(3) . .
O6 W2 O15 87.4(3) 6 .
O6 W2 O15 87.4(3) . .
O3 W3 O18 103.4(4) . .
O3 W3 O12 99.0(4) . .
O18 W3 O12 98.1(3) . .
O3 W3 O13 94.7(4) . .
O18 W3 O13 90.2(4) . .
O12 W3 O13 161.9(3) . .
O3 W3 O8 91.6(4) . .
O18 W3 O8 163.6(3) . .
O12 W3 O8 85.9(3) . .
O13 W3 O8 81.9(4) . .
O3 W3 O16 162.3(4) . .
O18 W3 O16 90.9(3) . .
O12 W3 O16 89.1(3) . .
O13 W3 O16 74.6(3) . .
O8 W3 O16 73.2(3) . .
O4 W4 O19 103.0(4) . .
O4 W4 O14 100.6(5) . .
O19 W4 O14 90.5(4) . .
O4 W4 O13 97.2(4) . .
O19 W4 O13 90.0(4) . .
O14 W4 O13 161.5(4) . .
O4 W4 O9 93.9(4) . .
O19 W4 O9 163.0(3) . .
O14 W4 O9 87.5(4) . .
O13 W4 O9 86.6(4) . .
O4 W4 O16 165.9(4) . .
O19 W4 O16 88.7(3) . .
O14 W4 O16 86.9(4) . .
O13 W4 O16 74.6(3) . .
O9 W4 O16 74.4(3) . .
O5 W5 O17 101.9(4) . 5_765
O5 W5 O12 99.1(4) . .
O17 W5 O12 90.2(3) 5_765 .
O5 W5 O11 98.5(4) . .
O17 W5 O11 92.8(4) 5_765 .
O12 W5 O11 161.2(4) . .
O5 W5 O10 93.4(4) . .
O17 W5 O10 164.7(3) 5_765 .
O12 W5 O10 86.9(3) . .
O11 W5 O10 85.3(4) . .
O5 W5 O15 166.0(4) . .
O17 W5 O15 90.5(4) 5_765 .
O12 W5 O15 87.2(3) . .
O11 W5 O15 74.3(3) . .
O10 W5 O15 74.3(4) . .
O20 Zn1 O16 114.6(3) 5_765 6
O20 Zn1 O16 114.6(3) 5_765 .
O16 Zn1 O16 104.0(5) 6 .
O20 Zn1 O15 110.8(5) 5_765 .
O16 Zn1 O15 106.1(3) 6 .
O16 Zn1 O15 106.1(3) . .
O19 Zn2 O19 177.6(4) . 2_765
O19 Zn2 O18 95.1(3) . 2_765
O19 Zn2 O18 86.5(3) 2_765 2_765
O19 Zn2 O18 86.5(3) . .
O19 Zn2 O18 95.1(3) 2_765 .
O18 Zn2 O18 98.2(4) 2_765 .
O19 Zn2 O20 97.0(4) . 5_765
O19 Zn2 O20 81.2(4) 2_765 5_765
O18 Zn2 O20 165.5(4) 2_765 5_765
O18 Zn2 O20 90.6(3) . 5_765
O19 Zn2 O20 81.2(4) . .
O19 Zn2 O20 97.0(4) 2_765 .
O18 Zn2 O20 90.6(3) 2_765 .
O18 Zn2 O20 165.5(4) . .
O20 Zn2 O20 83.3(4) 5_765 .
O19 Zn2 Bi1 44.7(2) . .
O19 Zn2 Bi1 133.7(2) 2_765 .
O18 Zn2 Bi1 88.0(2) 2_765 .
O18 Zn2 Bi1 131.3(2) . .
O20 Zn2 Bi1 94.9(2) 5_765 .
O20 Zn2 Bi1 37.1(3) . .
O19 Zn2 Bi1 133.7(2) . 5_765
O19 Zn2 Bi1 44.7(2) 2_765 5_765
O18 Zn2 Bi1 131.3(2) 2_765 5_765
O18 Zn2 Bi1 88.0(2) . 5_765
O20 Zn2 Bi1 37.1(3) 5_765 5_765
O20 Zn2 Bi1 94.9(2) . 5_765
Bi1 Zn2 Bi1 123.09(5) . 5_765
O20 Bi1 O17 87.0(3) . .
O20 Bi1 O17 87.0(3) . 6
O17 Bi1 O17 86.0(4) . 6
O20 Bi1 O19 75.9(3) . .
O17 Bi1 O19 162.9(3) . .
O17 Bi1 O19 93.7(3) 6 .
O20 Bi1 O19 75.9(3) . 6
O17 Bi1 O19 93.7(3) . 6
O17 Bi1 O19 162.9(3) 6 6
O19 Bi1 O19 81.6(4) . 6
O20 Bi1 Zn2 38.07(19) . .
O17 Bi1 Zn2 124.7(2) . .
O17 Bi1 Zn2 85.36(19) 6 .
O19 Bi1 Zn2 38.4(2) . .
O19 Bi1 Zn2 80.76(19) 6 .
O20 Bi1 Zn2 38.07(19) . 5_765
O17 Bi1 Zn2 85.36(19) . 5_765
O17 Bi1 Zn2 124.7(2) 6 5_765
O19 Bi1 Zn2 80.76(19) . 5_765
O19 Bi1 Zn2 38.4(2) 6 5_765
Zn2 Bi1 Zn2 56.91(5) . 5_765
W5 O5 Na1 138.7(5) . 3_645
W1 O6 W2 153.1(5) . .
W1 O7 W1 154.9(7) . 6
W1 O8 W3 112.9(4) . .
W1 O9 W4 114.3(4) . .
W1 O9 Na1 113.6(4) . .
W4 O9 Na1 118.8(5) . .
W2 O10 W5 114.1(3) . .
W5 O11 W5 111.7(5) . 6
W3 O12 W5 148.5(4) . .
W4 O13 W3 110.5(3) . .
W4 O14 W4 154.0(6) 6 .
Zn1 O15 W5 118.0(3) . .
Zn1 O15 W5 118.0(3) . 6
W5 O15 W5 98.5(4) . 6
Zn1 O15 W2 122.7(5) . .
W5 O15 W2 97.3(3) . .
W5 O15 W2 97.3(3) 6 .
Zn1 O16 W3 115.2(4) . .
Zn1 O16 W4 120.0(4) . .
W3 O16 W4 98.5(3) . .
Zn1 O16 W1 122.7(4) . .
W3 O16 W1 98.8(3) . .
W4 O16 W1 96.9(3) . .
W5 O17 Bi1 139.2(4) 5_765 .
W3 O18 Zn2 141.0(4) . .
W4 O19 Zn2 140.3(4) . .
W4 O19 Bi1 119.7(4) . .
Zn2 O19 Bi1 96.8(3) . .
Zn1 O20 Bi1 121.6(5) 5_765 .
Zn1 O20 Zn2 112.8(4) 5_765 .
Bi1 O20 Zn2 104.8(4) . .
Zn1 O20 Zn2 112.8(4) 5_765 5_765
Bi1 O20 Zn2 104.8(4) . 5_765
Zn2 O20 Zn2 96.7(4) . 5_765
Zn3A Zn3 O22 112.6(14) . 8_766
Zn3A Zn3 O22 112.6(14) . 3_655
O22 Zn3 O22 112.1(17) 8_766 3_655
Zn3A Zn3 O23 118.5(13) . .
O22 Zn3 O23 100.0(11) 8_766 .
O22 Zn3 O23 100.0(11) 3_655 .
Zn3A Zn3 O24 48.8(7) . 6_556
O22 Zn3 O24 161.4(14) 8_766 6_556
O22 Zn3 O24 79.4(12) 3_655 6_556
O23 Zn3 O24 92.0(8) . 6_556
Zn3A Zn3 O24 48.8(7) . .
O22 Zn3 O24 79.4(12) 8_766 .
O22 Zn3 O24 161.4(14) 3_655 .
O23 Zn3 O24 92.0(8) . .
O24 Zn3 O24 86.0(10) 6_556 .
Zn3A Zn3 O22A 131.9(11) . 8_766
O22 Zn3 O22A 19.4(7) 8_766 8_766
O22 Zn3 O22A 100.8(16) 3_655 8_766
O23 Zn3 O22A 86.9(9) . 8_766
O24 Zn3 O22A 178.9(10) 6_556 8_766
O24 Zn3 O22A 94.0(10) . 8_766
Zn3A Zn3 O22A 131.9(11) . 3_655
O22 Zn3 O22A 100.8(16) 8_766 3_655
O22 Zn3 O22A 19.4(7) 3_655 3_655
O23 Zn3 O22A 86.9(9) . 3_655
O24 Zn3 O22A 94.0(10) 6_556 3_655
O24 Zn3 O22A 178.9(10) . 3_655
O22A Zn3 O22A 85.9(17) 8_766 3_655
Zn3A Zn3 O31A 172.0(13) . 3_655
O22 Zn3 O31A 71.1(14) 8_766 3_655
O22 Zn3 O31A 71.1(14) 3_655 3_655
O23 Zn3 O31A 53.5(9) . 3_655
O24 Zn3 O31A 127.5(6) 6_556 3_655
O24 Zn3 O31A 127.5(6) . 3_655
O22A Zn3 O31A 51.7(10) 8_766 3_655
O22A Zn3 O31A 51.7(10) 3_655 3_655
Zn3A Zn3 O26 56.4(12) . .
O22 Zn3 O26 82.8(12) 8_766 .
O22 Zn3 O26 82.8(11) 3_655 .
O23 Zn3 O26 174.9(9) . .
O24 Zn3 O26 84.2(7) 6_556 .
O24 Zn3 O26 84.2(7) . .
O22A Zn3 O26 96.9(8) 8_766 .
O22A Zn3 O26 96.9(8) 3_655 .
O31A Zn3 O26 131.6(9) 3_655 .
Zn3 Zn3A O24 100.4(12) . 6_556
Zn3 Zn3A O24 100.4(12) . .
O24 Zn3A O24 126(2) 6_556 .
Zn3 Zn3A O26 97.4(15) . .
O24 Zn3A O26 112.8(11) 6_556 .
O24 Zn3A O26 112.8(11) . .
Zn3 Zn3A O24A 123.6(10) . 6_556
O24 Zn3A O24A 23.3(9) 6_556 6_556
O24 Zn3A O24A 113.0(15) . 6_556
O26 Zn3A O24A 108.7(11) . 6_556
Zn3 Zn3A O24A 123.6(10) . .
O24 Zn3A O24A 113.0(15) 6_556 .
O24 Zn3A O24A 23.3(9) . .
O26 Zn3A O24A 108.7(11) . .
O24A Zn3A O24A 94.4(15) 6_556 .
Zn3 Zn3A Na1 95.1(7) . .
O24 Zn3A Na1 54.1(9) 6_556 .
O24 Zn3A Na1 163.8(14) . .
O26 Zn3A Na1 60.2(3) . .
O24A Zn3A Na1 60.6(6) 6_556 .
O24A Zn3A Na1 141.3(11) . .
Zn3 Zn3A Na1 95.1(7) . 6_556
O24 Zn3A Na1 163.8(14) 6_556 6_556
O24 Zn3A Na1 54.1(9) . 6_556
O26 Zn3A Na1 60.2(3) . 6_556
O24A Zn3A Na1 141.3(11) 6_556 6_556
O24A Zn3A Na1 60.6(6) . 6_556
Na1 Zn3A Na1 120.2(6) . 6_556
O9 Na1 Na1 106.5(4) . 2_665
O9 Na1 O22 88.0(6) . 3_655
Na1 Na1 O22 138.2(6) 2_665 3_655
O9 Na1 O5 116.3(5) . 3_655
Na1 Na1 O5 123.1(6) 2_665 3_655
O22 Na1 O5 80.5(5) 3_655 3_655
O9 Na1 Zn3A 109.5(5) . .
Na1 Na1 Zn3A 93.9(4) 2_665 .
O22 Na1 Zn3A 44.6(6) 3_655 .
O5 Na1 Zn3A 104.5(5) 3_655 .
O22A O22 Zn3 90(3) . 3_645
O22A O22 Na1 162(3) . 3_645
Zn3 O22 Na1 107.5(17) 3_645 3_645
O22 O22A Zn3 70(2) . 3_645
O24A O24 Zn3A 121(2) . .
O24A O24 Zn3 151.7(19) . .
Zn3A O24 Zn3 30.8(9) . .
O24 O24A Zn3A 35.3(14) . .
Zn3A O26 Zn3 26.2(7) . .
O31 O31A Zn3 173(3) . 3_645
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O1 1.737(10) .
W1 O8 1.881(9) .
W1 O7 1.914(3) .
W1 O6 1.915(8) .
W1 O9 1.923(9) .
W1 O16 2.235(8) .
W2 O2 1.731(12) .
W2 O10 1.909(8) 6
W2 O10 1.909(8) .
W2 O6 1.922(8) 6
W2 O6 1.922(8) .
W2 O15 2.241(11) .
W3 O3 1.745(9) .
W3 O18 1.764(8) .
W3 O12 1.924(8) .
W3 O13 2.004(8) .
W3 O8 2.095(9) .
W3 O16 2.132(8) .
W4 O4 1.727(9) .
W4 O19 1.849(9) .
W4 O14 1.942(3) .
W4 O13 1.960(8) .
W4 O9 2.001(9) .
W4 O16 2.169(7) .
W5 O5 1.729(8) .
W5 O17 1.804(8) 5_765
W5 O12 1.935(8) .
W5 O11 1.969(6) .
W5 O10 2.019(8) .
W5 O15 2.151(7) .
Zn1 O20 1.934(11) 5_765
Zn1 O16 1.944(8) 6
Zn1 O16 1.944(8) .
Zn1 O15 1.954(10) .
Zn2 O19 2.085(8) .
Zn2 O19 2.085(8) 2_765
Zn2 O18 2.097(7) 2_765
Zn2 O18 2.097(7) .
Zn2 O20 2.125(7) 5_765
Zn2 O20 2.125(7) .
Zn2 Bi1 3.3320(10) .
Zn2 Bi1 3.3320(10) 5_765
Bi1 O20 2.079(10) .
Bi1 O17 2.255(8) .
Bi1 O17 2.255(8) 6
Bi1 O19 2.363(8) .
Bi1 O19 2.363(8) 6
Bi1 Zn2 3.3320(10) 5_765
O5 Na1 2.817(12) 3_645
O7 W1 1.914(3) 6
O9 Na1 2.689(14) .
O11 W5 1.969(6) 6
O14 W4 1.942(3) 6
O15 W5 2.151(7) 6
O17 W5 1.804(8) 5_765
O20 Zn1 1.934(11) 5_765
O20 Zn2 2.125(7) 5_765
Zn3 Zn3A 1.08(2) .
Zn3 O22 1.979(17) 8_766
Zn3 O22 1.979(17) 3_655
Zn3 O23 2.00(2) .
Zn3 O24 2.077(18) 6_556
Zn3 O24 2.077(18) .
Zn3 O22A 2.10(2) 8_766
Zn3 O22A 2.10(2) 3_655
Zn3 O31A 2.40(3) 3_655
Zn3 O26 2.43(3) .
Zn3A O24 1.589(19) 6_556
Zn3A O24 1.589(19) .
Zn3A O26 2.04(3) .
Zn3A O24A 2.35(3) 6_556
Zn3A O24A 2.35(3) .
Zn3A Na1 3.677(15) .
Zn3A Na1 3.677(15) 6_556
Na1 Na1 2.76(2) 2_665
Na1 O22 2.85(5) 3_655
Na1 O5 2.817(12) 3_655
O22 O22A 0.70(2) .
O22 Zn3 1.979(17) 3_645
O22 Na1 2.85(5) 3_645
O22A Zn3 2.10(2) 3_645
O24 O24A 1.09(3) .
O27 O27A 0.69(4) .
O31 O31A 1.00(3) .
O31A Zn3 2.40(3) 3_645
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O17 W5 O5 Na1 -137.6(7) 5_765 3_645
O12 W5 O5 Na1 130.3(7) . 3_645
O11 W5 O5 Na1 -43.0(8) . 3_645
O10 W5 O5 Na1 42.8(8) . 3_645
O15 W5 O5 Na1 15(2) . 3_645
O1 W1 O8 W3 -174.0(4) . .
O7 W1 O8 W3 13.0(14) . .
O6 W1 O8 W3 84.8(4) . .
O9 W1 O8 W3 -76.8(4) . .
O16 W1 O8 W3 -3.7(3) . .
O3 W3 O18 Zn2 -148.2(6) . .
O12 W3 O18 Zn2 110.5(7) . .
O13 W3 O18 Zn2 -53.4(7) . .
O8 W3 O18 Zn2 7.5(16) . .
O16 W3 O18 Zn2 21.2(7) . .
O4 W4 O19 Zn2 147.3(7) . .
O14 W4 O19 Zn2 -111.7(7) . .
O13 W4 O19 Zn2 49.9(7) . .
O9 W4 O19 Zn2 -28.6(17) . .
O16 W4 O19 Zn2 -24.7(7) . .
O4 W4 O19 Bi1 -58.5(5) . .
O14 W4 O19 Bi1 42.6(5) . .
O13 W4 O19 Bi1 -155.9(4) . .
O9 W4 O19 Bi1 125.6(11) . .
O16 W4 O19 Bi1 129.5(4) . .
O22 Zn3 Zn3A O24 178.9(12) 8_766 6_556
O22 Zn3 Zn3A O24 51.0(16) 3_655 6_556
O23 Zn3 Zn3A O24 -65.1(12) . 6_556
O24 Zn3 Zn3A O24 -130(2) . 6_556
O22A Zn3 Zn3A O24 -178.8(11) 8_766 6_556
O22A Zn3 Zn3A O24 49(2) 3_655 6_556
O26 Zn3 Zn3A O24 114.9(12) . 6_556
O22 Zn3 Zn3A O24 -51.0(16) 8_766 .
O22 Zn3 Zn3A O24 -178.9(12) 3_655 .
O23 Zn3 Zn3A O24 65.1(12) . .
O24 Zn3 Zn3A O24 130(2) 6_556 .
O22A Zn3 Zn3A O24 -49(2) 8_766 .
O22A Zn3 Zn3A O24 178.8(11) 3_655 .
O26 Zn3 Zn3A O24 -114.9(12) . .
O22 Zn3 Zn3A O26 64.0(8) 8_766 .
O22 Zn3 Zn3A O26 -64.0(8) 3_655 .
O23 Zn3 Zn3A O26 180.0 . .
O24 Zn3 Zn3A O26 -114.9(12) 6_556 .
O24 Zn3 Zn3A O26 114.9(12) . .
O22A Zn3 Zn3A O26 66.3(11) 8_766 .
O22A Zn3 Zn3A O26 -66.3(11) 3_655 .
O22 Zn3 Zn3A O24A -177.7(12) 8_766 6_556
O22 Zn3 Zn3A O24A 54.4(19) 3_655 6_556
O23 Zn3 Zn3A O24A -61.7(14) . 6_556
O24 Zn3 Zn3A O24A 3.4(11) 6_556 6_556
O24 Zn3 Zn3A O24A -127(2) . 6_556
O22A Zn3 Zn3A O24A -175.4(10) 8_766 6_556
O22A Zn3 Zn3A O24A 52(2) 3_655 6_556
O26 Zn3 Zn3A O24A 118.3(14) . 6_556
O22 Zn3 Zn3A O24A -54.4(19) 8_766 .
O22 Zn3 Zn3A O24A 177.7(12) 3_655 .
O23 Zn3 Zn3A O24A 61.7(14) . .
O24 Zn3 Zn3A O24A 127(2) 6_556 .
O24 Zn3 Zn3A O24A -3.4(11) . .
O22A Zn3 Zn3A O24A -52(2) 8_766 .
O22A Zn3 Zn3A O24A 175.4(10) 3_655 .
O26 Zn3 Zn3A O24A -118.3(14) . .
O22 Zn3 Zn3A Na1 124.5(7) 8_766 .
O22 Zn3 Zn3A Na1 -3.4(11) 3_655 .
O23 Zn3 Zn3A Na1 -119.5(4) . .
O24 Zn3 Zn3A Na1 -54.4(10) 6_556 .
O24 Zn3 Zn3A Na1 175.5(15) . .
O22A Zn3 Zn3A Na1 126.8(9) 8_766 .
O22A Zn3 Zn3A Na1 -5.7(15) 3_655 .
O26 Zn3 Zn3A Na1 60.5(4) . .
O22 Zn3 Zn3A Na1 3.4(11) 8_766 6_556
O22 Zn3 Zn3A Na1 -124.5(7) 3_655 6_556
O23 Zn3 Zn3A Na1 119.5(4) . 6_556
O24 Zn3 Zn3A Na1 -175.5(15) 6_556 6_556
O24 Zn3 Zn3A Na1 54.4(10) . 6_556
O22A Zn3 Zn3A Na1 5.7(15) 8_766 6_556
O22A Zn3 Zn3A Na1 -126.8(9) 3_655 6_556
O26 Zn3 Zn3A Na1 -60.5(4) . 6_556
Na1 O22 O22A Zn3 -178(10) 3_645 3_645
Zn3 Zn3A O24 O24A -173(2) . .
O24 Zn3A O24 O24A -62(4) 6_556 .
O26 Zn3A O24 O24A 84(3) . .
O24A Zn3A O24 O24A -39(3) 6_556 .
Na1 Zn3A O24 O24A 24(6) . .
Na1 Zn3A O24 O24A 98(3) 6_556 .
O24 Zn3A O24 Zn3 111(3) 6_556 .
O26 Zn3A O24 Zn3 -102.7(18) . .
O24A Zn3A O24 Zn3 134(2) 6_556 .
O24A Zn3A O24 Zn3 173(2) . .
Na1 Zn3A O24 Zn3 -164(5) . .
Na1 Zn3A O24 Zn3 -88.7(13) 6_556 .
Zn3 O24 O24A Zn3A -8(3) . .
